VOLUME 88, NUMBER 9 P H Y S I C A L R E V I E W L E T T E R S 4 MARCH 2002
Absence of a Loss of In-Plane Infrared Spectral Weight in the Pseudogap Regimeof Bi2Sr2CaCu2O81d
A. F. Santander-Syro,1 R. P. S. M. Lobo,1 N. Bontemps,1 Z. Konstantinovic,2 Z. Li,2 and H. Raffy21Laboratoire de Physique du Solide, Ecole Suprieure de Physique et Chimie Industrielles de la Ville de Paris, CNRS UPR 5,
75231 Paris Cedex 5, France2Laboratoire de Physique des Solides, Universit Paris-Sud, 91405 Orsay cedex, France
(Received 6 July 2001; published 19 February 2002)
The ab-plane reflectance of Bi2Sr2CaCu2O81d (Bi-2212) thin films was measured in the30 25 000 cm21 range for one underdoped (Tc 70 K), and one overdoped sample (Tc 63 K) downto 10 K. We find similar behaviors in the temperature dependence of the normal-state infrared responseof both samples. Above Tc , the effective spectral weight, obtained from the integrated conductivity,does not decrease when T decreases, so that no opening of an optical pseudogap is seen. We suggestthat these are consequences of the pseudogap opening in the k 0,p direction and of the in-planeinfrared conductivity being mostly sensitive to the k p,p direction.
DOI: 10.1103/PhysRevLett.88.097005 PACS numbers: 74.25.Gz, 72.15.v, 74.72.HsThe normal state of high-Tc superconductors, in particu-lar the pseudogap state, is highly debated . A numberof experiments in underdoped samples nuclear magneticresonance (NMR) , specific heat , uniform sus-ceptibility  show the opening of a gap in the densityof states at some temperature T . Tc. Similarly, Ra-man spectroscopy points to a depletion of scattered inten-sity at low energy . Nevertheless, the very existenceof T is disputed . Tunneling data exhibit a broad dipabove Tc , over the same energy range of the supercon-ducting gap. Angle-resolved photoemission spectroscopy(ARPES) measurements display a shift of the leading edgeof the energy dispersion curve spectrum in the 0,p direc-tion . They also show that significant arcs of the Fermisurface are still present in the p,p direction down toTc .
The in-plane dc resistivity in underdoped cuprates showsa deviation from the high temperature linear behavior.In Bi-2212, the temperature where this deviation occursagrees with T as determined by other techniques (NMR,ARPES) [11,12]. The real part s1v,T of the ab-planeinfrared (IR) conductivity of underdoped samples exhibitsa depression developing as T . Tc decreases within anenergy range extending typically from 200 to 1500 cm21
for the YBCO, Bi-2212, and Tl-2201 compounds .This loss of spectral weight (SW) was assigned either tothe pseudogap opening or to a shift of SW towards verylow frequencies . It is obviously difficult to discrimi-nate between these two approaches due to experimen-tal limitations in the low frequency part of the spectrum(usually restricted to v * 30 cm21). A suppression ofthe optical scattering rate 1tv in underdoped samplesbelow a typical constant energy scale 700 cm21, irre-spective of temperature and doping, was suggested to bethe infrared signature of the pseudogap state .None of these IR data convincingly defines a T due tothe small number of experimentally available tempera-tures .97005-1 0031-90070288(9)097005(4)$20.00Indeed, to the best of our knowledge, no systematicstudy of the detailed temperature dependence of thein-plane optical conductivity has been performed todate. In this work, we report such a study in Bi-2212thin films for a set of 15 temperatures. Thanks to theirhighly reflective surface and their large area (typically$5 3 5 mm2), thin films allow to resolve reliably relativechanges in reflectance as small as 0.2%. This unprece-dented accuracy allows us to look for the opening of apseudogap by tracking a transfer of spectral weight fromlow to high energies, possibly occurring below T . Tc.Our data rule out such a direct signature of a pseudogapin the IR response, as they show the opposite behavior,namely spectral weight is collected at low energies astemperature decreases.
Thin films of Bi-2212 were epitaxially grown by RFmagnetron sputtering onto SrTiO3 substrates. As thetemperature is decreased from room temperature, theirin-plane resistivity rab departs from an initial T-linearvariation, developing a slight positive curvature in theoverdoped case, and a negative one in the underdopedstates. The latter behavior occurs below a temperatureT , commonly assigned to the onset of a pseudogap.The phase diagram thus derived was entirely compatiblewith the one obtained from, e.g., ARPES measurementsin single crystals and similar films [17,18]. Our spectrawere recorded in (i) an underdoped (UD) film (thickness2400 ), with TcR 0 70 K, and a relatively broad(onset-offset) transition width 15 K, and T 170 K,according to the resisitivity curve, and (ii) an overdoped(OD) film (thickness 3000 ), with TcR 0 63 K,and a transition width 5 K.
Our data were collected with a Bruker IFS 66v interfer-ometer (30 7000 cm21). Near-infrared and visible data(4000 25 000 cm21) were measured in a Cary 5E gratingspectrometer. In the overlapping spectral range, measure-ments agree within 1.5%. The spectra were measured for15 temperatures between 300 and 10 K. A He gas flow 2002 The American Physical Society 097005-1
VOLUME 88, NUMBER 9 P H Y S I C A L R E V I E W L E T T E R S 4 MARCH 2002cryostat allows to stabilize the temperature within 60.2 K.Figure 1 shows the reflectivity of the two samples, for a re-stricted set of temperatures, up to 1500 cm21.
Studying thin films precludes the use of the Kramers-Kronig (KK) transform to obtain the conductivity, due tothe contribution of the substrate to the experimentally mea-sured reflectivity. Therefore, in order to derive the opticalconductivity of the films, we fit the reflectance of the filmon top of a substrate using an attempt dielectric functionfor the film, and the optical constants of SrTiO3 that wehave experimentally determined for each temperature. Themodel dielectric function that fits the reflectance involvesLorentz and Drude oscillators, thus warranting causality.The procedure is described in detail elsewhere [19,20].An interesting outcome of this approach is that it provideswhat can be considered our best guess for the extrapolationof the dielectric function in the energy range which is notavailable experimentally, i.e., v & 30 cm21.
A systematic error in the absolute value of the reflectiv-ity 60.5% is irrelevant since we are only interested in itsrelative changes with temperature. The change of a spec-trum versus temperature is defined within DTR # 0.2%,and the accuracy of the fit is DFR # 0.5%. This resultsin a typical error of 5% in the conductivity . Aftercompleting the fitting procedure, we obtain all the relevantspectral functions for the film. We show in Fig. 2(a) thereal part of the conductivity s1v,T for the UD sample,at the same temperatures as in Fig. 1. Figure 2(b) dis-plays similar results for the OD sample. The dc resisi-tivity derived from our s1v, T data are consistent withdc transport measurements on similar films. The so-called
0 500 1000 1500
(a) UD 10 K50 K80 K
100 K150 K200 K250 K
Wave number (cm-1)
FIG. 1. Reflectivity of (a) the underdoped and (b) the over-doped film. The sharp peaks at 550, 120, and below 100 cm21,especially visible in the underdoped sample, are the phononmodes of the substrate.097005-2pseudogap effect shows up in the UD sample [Fig. 2(a)]as a depression in the conductivity above Tc, in the range200 1500 cm21, as observed previously in single crys-tals. In the OD sample, a similar depletion of the con-ductivity occurs above Tc in the same spectral range. Thequestion is whether the observed loss is balanced by theincrease of spectral weight at low energy.
Before we address this point, we touch upon the scatter-ing rate, defined as
The plasma frequency Vp (in cm21) was obtained by in-tegrating s1v up to 1 eV. Z0 377 V is the vacuumimpedance. Taking sv in V21 cm21, one gets 1tvin cm21. 1tv is shown in the insets of Figs. 2(a) and2(b). As we are focusing on the normal state, we haveonly plotted 1tv above Tc. In the UD sample, whenthe temperature decreases, a gradual depletion of 1tvbelow 700 cm21 is observed [inset of Fig. 2(a)]. A simi-lar, less pronounced, depletion below the same energy isalso observed in the OD sample already above Tc [inset ofFig. 2(b)]. This fact can already be traced in those singlecrystals where doping was changed only by varying theamount of oxygen, and has been ascribed in the under-doped regime to the opening of an optical pseudogap .
Our data show distinctly the connection between the in-crease of the conductivity and the depression of the lowenergy scattering rate in both samples. The most strikingresult is the narrowing and increase of the low frequency
0 1000 2000 3000
0 1000 2000 30000
0 500 1000 1500 20000
Wave number (cm-1)
Wave number (cm-1)
Wave number (cm-1)
FIG. 2. Real part of the conductivity (from fit) of (a) the under-doped and (b) the overdoped film. The insets show the scatteringrate for T . Tc (see text), using Vp 16 000 and 16 600 cm21,respectively. The line types refer to the same temperatures asin Fig. 1. The conductivity extrapolated from 30 cm21 down tozero results from the fit (see text).097005-2
VOLUME 88, NUMBER 9 P H Y S I C A L R E V I E W L E T T E R S 4 MARCH 2002Drude-like peak in the UD sample conductivity occuring inthe superconducting state, with no obvious loss of spectralweight associated with the formation of the condensate. Incontrast, in the OD sample, the conductivity drops belowTc, and the missing area is clearly visible. The supercon-ducting state is discussed elsewhere .
Since a set of 15 temperatures is available, we can lookfor a loss of spectral weight as the temperature is lowered.This would be the actual signature of a pseudogap open-ing in the vicinity of the Fermi level. We have thereforeintegrated the conductivity in order to derive an effectivecarrier density up to vM , according to
Neff ~Z vM01
s1v dv . (2)
In order to display the thermal evolution starting fromroom temperature for various vM in a single plot, we havenormalized NeffvM ,T with respect to NeffvM , 300 K.We show in Fig. 3, for both samples, the temperaturevariation of this normalized effective carrier density(equivalent to a normalized SW) for a set of vM valuesspanning the full experimental frequency range. WhenvM 100 cm21, the SW increases sharply as the tem-perature decreases down to Tc, showing that spectralweight is collected at low frequency in the normal state.As vM is increased, the transfer of SW becomes lessapparent. The data for vM 5000 and 10 000 cm21 (notshown) can hardly be distinguished from those for
0 50 100 150 200 250 300
0 50 100 150 200 250 3001.0
) / N
FIG. 3. Spectral weight versus temperature for (a) the under-doped and (b) the overdoped film. Different symbols referto different cutoff frequencies vM . The inset shows the ef-fect of starting the integration from 0, 30, and 50 cm21 (up tovM 1000 cm21).097005-320 000 cm21. This shows that SW going to low frequencyvM , 100 cm21 comes mostly from the midinfraredrange. The most important conclusion is that, for de-creasing T , and for all vM values considered (up to20 000 cm21), there is a systematic increase of thespectral weight, both in the UD and OD samples. Thisobservation is at odds with the opening of a pseudogapwhich would yield a decrease of SW. Note that a breakin this trend of increasing SW as T decreases is seen onlyat the superconducting transition, where the SW hardlydecreases in the UD sample, and drops sharply in the ODsample (Fig. 3) .
So far, we have integrated Eq. (2) starting at zero fre-quency, using the computed s1v for v , 30 cm21. Inorder to check the sensitivity of our results to a low fre-quency cutoff, we have done a similar calculation, startingthe integration from 30 and from 50 cm21. The result forthe UD case is shown for vM 1000 cm21 in the insetof Fig. 3. Introducing a low frequency cutoff results in adecrease of SW already at T & 100 K, and a broad maxi-mum develops in temperature as the cutoff is increased.A similar behavior is observed for the overdoped sample.This being an artifact, confirms that no detectable loss ofSW is seen, making it impossible to locate T from thethermal evolution of the effective carrier density. Actually,from all the observations described above, it is clear thatthere is enough room in the low frequency part of the spec-trum to balance the small depression of spectral weight ob-served in the conductivity data. Our data strongly suggestthat the pseudogap has no clear-cut signature in the in-frared conductivity. Both the depletion in the scatteringrate and the occurrence of a narrow peak in the real part ofthe conductivity are settling gradually as the temperatureis decreased.
Since the existence of a pseudogap is establishedthrough a variety of experimental techniques, in boththe spin and the charge channels, why does the opticalconductivity appear not to display this phenomenon? Onelogical hypothesis is that the conductivity probes mostlythe quasiparticles (QPs) along the p ,p direction,where no pseudogap opens [9,10]. Indeed, recent ARPESexperiments on optimally doped Bi-2212 suggest that,as single-particle scattering rates near the nodes andtransport rates exhibit similar energy and temperaturedependencies, the in-plane transport might be dominatedby nodal excitations [23,24].
One may explore how reasonable the above hypothesis isin a simple framework. In the semiclassical approximation,the finite-frequency conductivity is :
sv ~Z y2k
t21k 2 iv
d2k , (3)
vk and k are the carrier bare (band-structural) veloc-ity and energy, respectively. t21k is the transportscattering rate, and f is the Fermi distribution function.As the derivative of f is peaked at the Fermi energy,097005-3
VOLUME 88, NUMBER 9 P H Y S I C A L R E V I E W L E T T E R S 4 MARCH 2002the integration in Eq. (3) over the direction perpendicularto the Fermi surface (FS) shows that a critical weight-ing factor is the bare Fermi velocity vF , whichdue tothe anisotropy of the FS is smaller in the k 0,pthan in the k p,p direction. Simple calculationsyield yFp,pyF 0,p 5 [26,27]. As a consequence,s1v should be mostly sensitive to the nodal QPs, andno pseudogap can be seen. Furthermore, as the anisotropyof the FS holds in a sizable doping range, the trends inthe T dependence of the normal-state s1v should notstrongly depend on doping. T...